RF Reactive Sputter Deposition and
RF Reactive Sputter Deposition and Characterization
im Fachbereich 07 (Physik) der Justus-Liebig-Universität Gießen
zur Erlangung des akademischen Grades Dr. rer. nat.
Prof. Dr. Bruno K. Meyer
Prof. Dr. Claus-Dieter Kohl
I. Physikalisches Institut
materials and properties: a brief review……….….5
2.1 Crystal structure ...5
2.2 Physical properties ...8
2.2.1 Electronic and optical properties...8
2.2.2 Electrical properties...10
Radio frequency sputtering: principle and film deposition ...13
3.1 Sputtering principle and apparatus...13
3.2 Film deposition ...15
Characterization methods: principles and instruments...19
4.1 Structural characterization methods (XRD, XRR, and TEM) ...19
4.1.1 X-ray diffraction...19
4.1.2 X-ray reflectometry ...23
4.1.3 Transmission electron microscopy...25
4.2 Surface and morphology characterization methods (XPS, UPS, SIMS, SEM, and AFM) ...25
4.2.1 Photoemission spectroscopy (XPS and UPS) ...25
4.2.2 Secondary ion mass spectrometry ...26
4.2.3 Scanning electron microscopy ...27
4.2.4 Atomic force microscopy ...28
4.3 Optical transmission...29
4.4 Hall effect measurements...29
One-stage deposition of CuInS2
films by RF reactive sputtering ...31
5.1 Influence of the sputter parameters on the properties of CuInS2 films ...31
5.1.1 Influence of the H2S flow during sputtering ...31
5.1.3 Influence of the sputter power...37
5.1.4 Effect of coating the substrate...37
5.1.5 Conclusions ...39
5.2 Surface characterization of one-step sputtered CuInS2 films ...41
5.2.1 Chemical analysis and valence band structure by photoemission spectroscopy (XPS and UPS) ...41
5.2.2 Surface morphology by AFM ...45
5.2.3 Surface segregation analysis by SEM and EDX...47
5.2.4 Surface structural properties by GIXRD and XRR...48
5.2.5 Surface survey and depth profile by SIMS...50
5.2.6 Conclusions ...52
5.3 Post-growth treatment effects on properties of the sputtered CuInS2 films...53
5.3.1 Post-growth annealing effect on the structural and optical properties...53
184.108.40.206 Annealing with H2S ...54
220.127.116.11 Annealing under vacuum ...55
5.3.2 Chemical etching of CuxS segregation by KCN...57
5.3.3 Aging and etching effects on the electrical properties...59
5.3.4 Conclusions ...63
Quasi-epitaxial growth of CuInS2
films on sapphire ...65
6.1 Heteroepitaxial growth of very thin CuInS2 films on sapphire...66
6.2 Quasi-epitaxial growth of thick CuInS2 films...75
6.2.1 Structural characteristics of the thick CuInS2 films sputtered directly on sapphire...75
6.2.2 Quasi-epitaxial growth of thick CuInS2 films on an ultrathin buffer-layer77 6.3 Transmission electron microscopy characterization on quasi-epitaxially grown CuInS2 films ...85
Summary and outlook...87
Curriculum vitae ...115
As the environmental and energy resource concerns have become more and more imperative, great efforts have been put in the development of renewable energy resources, among which photovoltaic solar power is the most desirable one and holds great potential and promise.
Photovoltaic (PV) solar power converts directly the sunlight to electricity by using the photovoltaic effect, which was discovered in 1839 by Edmond Becquerel . Compared to nonrenewable sources such as coal, gas, oil, and nuclear, the advantages of the PV solar power are clear: its source is entirely safe, free of charge, and non-exhausting, given a no-end life of the sun, and the power generation is totally non-polluting, i.e., causing no changes to the environment when generating power. Even compared to other renewable energy sources such as wind power, water power, and solar thermal power, PV solar power holds obvious advantages. Whereas wind and water electrical power generation, relying on turbines to turn generators with moving parts, are noisy and require maintenance, PV systems, with no moving parts, require virtually no maintenance, and have cells that can last for decades. In addition, the exclusive modular nature of PV enables designers to build PV systems with various power output in a distributed fashion, and allowing the power generation to keep in step with growing needs without having to overbuild generation capacity as is often the case with conventional large scale power systems. Since its first commercial use in powering orbital satellites in the 1950s, PV has been widely used in space and on the earth for several decades. Today’s PV market is about 381 MW (in 2001) corresponding to a value of over US$1.4 billion .
Crystalline silicon was first used to produce PV cells (also known as solar cells), and still dominates the PV market today. This is mostly due to a well-established knowledge on silicon material science and engineering, an available abundant supply of silicon raw material, and the advantages of low ecological impact but high efficiencies. However, the relatively high price of crystalline silicon material, and additionally its too low optical absorption (~102 cm-1), due to an indirect transition, requiring a much larger raw material consumption and a complicated manufacturing, lead to a high installation cost for crystalline silicon-based PV technology. From this point of view, the PV power generation is not competitive in most urban areas where conventionally generated power is readily available. A substantial reduction of PV production costs is expected from the development of thin film solar cells, in which highly absorption layers with a few micrometer thickness can be produced by economical, high-volume manufacturing techniques. This lays down the background for the extensive research interest in materials
suitable for thin film solar cells. At present, several manufacturing facilities based on a-Si, CdTe, and CuInSe2 are in the pilot-line stage. The latest developments in the field of thin
film solar cells can be found in the recently published review articles [3-5].
I-III-VI2 compounds, especially Cu-chalcopyrite thin films have played a major role in
thin film PV technology. Typical Cu-chalcopyrite-based absorber materials are CuInSe2,
CuInS2, CuGaSe2 and their alloys with bandgaps ranging from 1.05 to 1.7 eV, which is
favorable for absorbing the solar radiation. The high absorption coefficient of these materials of almost 105 cm-1 assures a complete absorption of the incident photon flux in an absorber layer as thin as a few microns. Polycrystalline chalcopyrite-based thin film solar cells have recently reached conversion efficiencies as high as 18.8%, which is the highest value so far achieved for any polycrystalline thin film solar cell. This record device consists basically of a coevaporation-deposited p-type Cu(InGa)Se2 absorber layer, an
n-type thin CdS buffer, and an n-n-type ZnO window layer .
Compared to other selenium chalcopyrites such as CuInSe2, CuInS2 is even more
favorable for PV solar power. Substituting the problematic selenium by non-toxic sulfur, CuInS2 is more environment-friendly than CuInSe2. The open circuit voltage of CuInS2
solar cells is theoretically higher than that of CuInSe2 and Cu(InGa)Se2-based solar cells.
Its photo current is lower, which is advantageous for the serial connection of multiple cells in a module. Due to a superior bandgap of about 1.5 eV, matching almost ideally to the solar spectrum, CuInS2 has in principle the highest conversion efficiency among the
Cu-chalcopyrite-based solar cells [7, 8]. However, the efficiency of CuInS2 solar cells is so far
limited by the open circuit voltage that is far below the theoretical value. The best conversion efficiency for polycrystalline CuInS2 solar cells achieved to date is 12.7% [9,
10], considerably lower than that of cells based on CuInSe2 (14.8%)  and Cu(InGa)Se2
(18.8%) . To improve further the solar cells’ efficiencies a better understanding on the absorber itself is essential. Whereas CuInSe2 has been widely studied for more than two
decades, CuInS2, especially as a thin film, has just attracted more attention recently. Great
potential but limited material knowledge motivated us to focus the present study on CuInS2
Up to now, a number of methods have been performed to produce CuInS2 films, including a rapid thermal process , single source evaporation ,coevaporation from elemental sources ,sulfurization of metallic precursors ,chemical vapor deposition , sputtering , electrodeposition , and spray pyrolysis , etc. Among them, the sputtering technique holds in principle the advantage of simple and flexible control of the film stoichiometry over a large scale at relatively low cost. Its great potential for industrial application drove us to choose reactive sputtering as the technique for CuInS2
thin film deposition. Usually the deposition of CuInS2 film by sputtering consists of two
second step. Simplification of the process is one of the key issues for industrial application. In the present study, we demonstrate that CuInS2 films can be produced in one step by
radio frequency (RF) reactive sputtering with a Cu-In alloy target and H2S gas.
Normally a better understanding of the fundamental material properties can be expected from high-quality single-crystalline materials. However, it is well known that the controlled growth of high quality single crystals is a priori difficult for ternary compounds, and is additionally complicated by high temperature phase transitions that occur in many chalcopyrite compounds . It is therefore of great importance to achieve crystalline CuInS2 films e.g. by epitaxial growth. However, up to now such attempts have scarcely
been reported in the literature. With the molecular beam epitaxy (MBE) technique Metzner and Hahn successfully grew CuInS2 films heteroepitaxially on sulphur-terminated Si (111)
and Si (100) [19, 20], while Hunger achieved epitaxial growth of CuInS2 on
hydrogen-terminated Si (111) . In this work, we have succeeded in, to the best of our knowledge, the first epitaxial growth of CuInS2 films on (0001)-sapphire by RF reactive sputtering.
This thesis is organized as follows.
Chapter 2 starts with an introduction of the established crystalline structure of CuInS2,
followed by a brief summary of the known physical properties such as electrical, electronical, optical properties of CuInS2 material.
The working principle of the RF reactive sputter technique and the specific setup used in this work will shortly be described in Chapter 3.
Chapter 4 outlines the characterization techniques employed in this work, that is,
photoemission spectroscopy (XPS and UPS), secondary ion mass spectrometry (SIMS), X-ray diffraction (XRD), X-X-ray reflectometry (XRR), transmission electron microscopy (TEM), atomic force microscopy (AFM), and scanning electron microscopy (SEM) for surface, structure and morphology characterization, and optical transmission and Hall effect measurement for optical and electrical properties, respectively.
As a preliminary step, we used a Cu-In inlay target for sputtering, which leads to films with in general good structural properties but strong deficiency in the In content. By using a Cu-In alloy target instead, one-stage growth of stoichiometric CuInS2 films by RF
reactive sputtering has been achieved, as reported in Chapter 5. To optimize the sputtering process, in section 5.1, we first investigated systematically the influence of the sputter parameters on the film properties. Section 5.2 focuses on the characterization of the surface of the sputtered films, its knowledge is significant for achieving high-efficiency CuInS2
film solar cells. Although stoichiometric CuInS2 films can be sputtered in one step, it is
shown in section 5.3 that post-growth annealing improves significantly the properties of the sputtered films, and that the surface segregation of CuxS can be effectively removed by
post-growth chemical etching. Section 5.3 presents the post-treatment effects on the CuInS2 film properties.
In Chapter 6, the present work is highlighted by the success of epitaxial growth of CuInS2 films on crystalline (0001)-sapphire substrates. The structural characteristics of the
sputtered thin CuInS2 epilayers have been investigated, with special emphasis on
elucidating the origin for the epitaxial growth (section 6.1). With a thin epilayer as buffer, thick CuInS2 films grow quasi-epitaxially on sapphire. While the out-of-plane ordering of
the films is significantly enhanced, the in-plane alignment shows a multi-domain feature in contrast to films sputtered without the buffer. Section 6.2 discusses the structural properties of such thick films with special efforts on illustrating the role of the thin buffer layer. The TEM characterization of the sputtered quasi-epitaxially grown CuInS2 films is
presented in section 6.3.
Finally, a brief summary and an outlook for future work are drawn in English in
CuInS2 belongs to the family of ternary chalcopyrite compounds. In the early seventies a
comprehensive review of chalcopyrite compounds was first provided by Shay and Wernick . Whereas the earlier works were mainly on single crystalline specimens, motivated by their potential for non-linear optical applications, visible-light emitters, and photodetectors [2-5], the more recent experimental studies have been mostly devoted to thin films, due to their great perspectives for large area PV modules. The present work concentrates on the RF sputtering deposition and characterization of structural and physical properties such as electronical, optical, and electrical properties of CuInS2 thin films, aiming to establish a
sputtering-based method suitable for producing device grade CuInS2 absorber films. In this
chapter, a brief introduction to the well-established structural and physical properties of the material is provided as a basis for the analyses of the sputtered films, as will be presented in the following chapters in this study.
2.1 Crystal structure
The ternary chalcopyrite compounds AIBIIIXVI
2 (A=Cu, Ag; B=Al, Ga, In, Tl; and X=S, Se,
Te), similar with their isoelectronic II-VI binary analogues, derive from the tetrahedrally bounded class IV semiconductors. In the diamond structure of the class IV semiconductors, each atom has four neighbors situated at the corners of a regular tetrahedron bonded by hybridized sp3 bonds. In Fig. 2.1(c), a unit cell of CuInS
2 of the
chalcopyrite structure is illustrated, in comparison with the diamond (a) and zincblende (b) crystal structures. By arranging two units along a diagonal line through the cubes and shifting them, in terms of the basis vectors by (a/4, a/4, a/4) the diamond structure is created. The zincblende structure can be regarded as a superlattice structure of diamond, with one sublattice occupied by cations and the other by anions. In a ternary chalcopyrite structure whereas the anions remain at their sites the cations are furthermore replaced by one cation of lower valence (A) and one cation of higher valence (B) in the arrangement as shown in the figure.
The unique properties of the chalcopyrites are related to basically three structural differences with respect to the zincblende structure. Firstly, there are two cation sublattices
rather than one, leading to the existence of two basic chemical bonds A-X and B-X, in general with unequal bond lengths RAX ≠ RBX. Secondly, the unit cell is tetragonally
distorted with a distortion parameter η ≡ c/2a ≠ 1. Thirdly, the anions are displaced from the ideal tetrahedral site by an amount u . In the specific case of CuInS2 the Cu-S bond
length is 0.2335 nm, whereas the In-S one is 0.2464 nm . The sulfur atom moves away from the In atoms towards the Cu atoms, resulting in a stretched unit cell with η ≡ c/2a = 1.0065, associated with an anion displacement parameter u = 0.214 . The structural and electronic properties of the chalcopyrites are governed by the added structural (η, u) and chemical (A ≠ B) degrees of freedom relative to their binary analogues . Structural and optical properties of some typical chalcopyrite materials are compared in table 2.2.
Fig. 2.1. Structures of (a) diamond Si, (b) zincblende ZnS, (c) chalcopyrite CuInS2, and (d) CuAu ordered
CuInS2. Double unit cells are shown for (a) diamond Si, (b) zincblende ZnS, and (d) CuAu ordered CuInS2,
in comparison with the unit cell of chalcopyrite CuInS2.
The reduced symmetry, due to two kinds of cations, leads to a primitive cell of eight atoms in the chalcopyrite structure compared to a primitive cell of two atoms in the zincblende structure. The Bravais lattice of the chalcopyrite is body centered tetragonal, belonging to space group I 4 2d . Compared to the face centered cubic Bravais cell of
the zincblende the unit cell is doubled along the crystal c axis. At room temperature, the ternary compounds AIBIIIXVI2 stabilize in chalcopyrite, however, they may crystallize in
zincblende structure at high temperature (975-1047°C) where the different cations are distributed randomly .
The polymorphism is referred to the phenomenon that a solid with the same composition can appear in different crystal structures under different thermodynamical conditions. A set of polytypes of the chalcopyrite structure were theoretically constructed such that the electron counting rule is obeyed. By first-principles calculations Wei et al. determined the formation energies and band structures of CuInSe2 and CuInS2 polytypes
[11, 12]. It was shown that the CuAu-like ordered structure is the most likely to occur. An exceedingly small formation energy difference ∆Eform= -1.95 meV/atom was found
between chalcopyrite and CuAu-like phases of CuInS2. Similar results were obtained for
CuInSe2 where ∆Eform= -2.05 meV/atom. It was predicted that CuAu-like phases coexist in
nominally chalcopyrites CuInS2 and CuInSe2. Band gap energies are affected slightly by
the transition from chalcopyrite (CH) to polymorphous structures. Calculations resulted in
Eg (CH)-Eg (CuAu) = 30 meV for CuInS2 and in Eg (CH)-Eg (CuAu) = 46 meV for
CuInSe2. This suggests furthermore that formation of polytypes in these compounds has
insignificant effect on their electrical and optical properties.
An illustration of the CuAu-like structure is given in Fig. 2.1 (d) in comparison to the chalcopyrite structure. The anion sublattice is conserved in the CuAu structure and the cation order is changed such that the A2B2 coordination is conserved. The lattice type of the
CuAu-like structure is primitive tetragonal, corresponding to space group P 4 m2 . In table 2.1, chalcopyrite CuInS2 is compared to typical materials of diamond and zincblende
structures such as Si and ZnS, in terms of crystal structure, space group, Bravais lattice, and lattice constants.
Table 2.1 Summary of crystal structure, space group, Bravais lattice, and lattice constants of CuInS2 in the
Zincblende, chalcopyrite, and CuAu-like phases, in comparison with diamond Si and zincblende ZnS.
Material Crystal Structure Bravais Lattice Space Group Lattice Constants (nm) Si Diamond fcc Fd3m (227) a=b=c= 0.543  ZnS Zincblende fcc F43m (216) a=b=c= 0.5406  Zincblende fcc F43m (216) a=b=c= 0.551  Chalcopyrite bc-tetragonal I42d (122) a=b= 0.5523 c = 1.1133 c/2a = 1.0079 CuInS2
CuAu-like tetragonalprimitive P42m (111) a=b≈c
2.2 Physical properties
2.2.1 Electronic and optical properties
The electronic band structures of the typical Cu-based ternary chalcopyrite semiconductors including CuInS2 were theoretically studied by Jaffe and Zunger using a
density-function formalism and a first-principles all-electron band-structure approach [6, 17]. It has been concluded that the band gaps of Cu-III-VI2 chalcopyrites are controlled
essentially by two factors. The first one is a pure structural factor, caused by the tetragonal distortion, η = c/2a ≠ 1, and anion displacement from the ideal tetrahedral site, u ≠ 1/4, occurring in the chalcopyrite structure. These parameters, particularly u, determine the band gap in the system. Even a small increase of u from its ideal zincblende value results in a substantial ionic polarization of the bonds and consequently in a remarkable increase of the band gap. The effect of this factor in shown in table 2.2 where u is listed together with the band gap energies of six typical Cu-III-VI2 compounds.
The second one is an electronic factor. A great influence of the Cu 3d states on the valence band was found for Cu-III-VI2 chalcopyrites. These states hybridize with the p
states of the group VI components. As the d states are found in the upper half of the valence band they are responsible, in part, for the reduction of the band gap.
Table 2.2. List of the lattice constants a and c, the tetragonal distortion parameter η = c/2a, the anion displacement parameter u, and the observed lowest bandgaps at room temperature for typical Cu-III-VI2
compounds [6, 17]. Ternary Compound a = b (nm) c (nm) η u Eg (eV) CuInS2 0.5523 1.1118 1.0065 0.214 1.53 CuInSe2 0.5784 1.1614 1.004 0.224 1.04 CuGaSe2 0.5614 1.1032 0.9825 0.250 1.68 CuAlSe2 0.5602 1.0946 0.977 0.269 2.71 CuGaS2 0.5356 1.0433 0.974 0.275 2.43 CuAlS2 0.5334 1.0444 0.979 0.275 3.49
A schematic band structure of CuInS2 is shown in Fig. 2.2, with notation of the
contributions of the atomic orbitals. The valence band is separated into two parts, with the upper part reaching 5 eV and the lower one located around 7 eV. The Cu 3d and S 3p orbitals from the Cu-S bond contribute to the upper valence band whereas the S 3p and In 4p from the In-S bond form the lower valence band. At around 12 eV a band is built from S 3s states and a narrow band is set up near 17 eV by In 4d orbitals. The conduction band is
formed by S 3p and In 5s orbitals . This theoretical calculation of the band structure of CuInS2 is in good agreement with the experimental results of X-ray photoemission
spectroscopy in respect of the valence band structure [18, 19]. However, it underestimates the optical band gap relative to the experiment.
Fig. 2.2. Schematic band structure of CuInS2, with indication of contributions of the atomic orbitals and the
corresponding energy levels. Shade areas denote the major subbands, and the boxed numbers mark the three internal gaps .
Very recently, a detailed experimental work on optical functions and electronic structure of CuInS2 crystals was carried out by Alonso et al. using spectroscopic
ellipsometry . A more realistic band structure based on experiments was proposed there with assignments for the transitions observed in the optical range. In addition, optical parameters such as refraction index n and extinction coefficient k can be found there. In the present study, we consider the optical properties of the sputtered CuInS2 films mainly on
bandgap and absorption coefficient, which are essential for absorbing the solar radiation. CuInS2 is a direct semiconductor. Whereas bandgaps of 1.55 and 1.53 eV were found
for bulk single crystals at low (2 K) and room temperature, respectively, band gaps varying between 1.38 and 1.55 eV were reported for CuInS2 thin films at RT depending on
different deposition techniques used [1, 21-26]. As is normally expected for semiconductors, the bandgap of CuInS2 films decreases with increasing temperature and
can be characterized over the temperature range 300-77 K according to the relation ) /( 2 0−β +α =E T T Eg g (2.1)
with the initial bandgap Eg0=1.62 eV, two constants α =231.54 K and β = 4.3×10-4 eV/K,
respectively . Around the fundamental absorption edge, CuInS2 has an absorption
coefficient between 104 to 105 cm-1, it can thus absorb the incident light with photon energies higher than the bandgap within a few microns.
2.2.2 Electrical properties
A number of studies on the electrical properties of CuInS2 bulk single crystals and thin
films have been reported [27-32]. Unlike its binary II-VI analogues that are normally n-type, CuInS2 can be made both n- and p-type, depending upon its composition, i.e.,
deviation from molecularity and stoichiometry, defined as [Cu]/[In]-1 and 2[S]/([Cu]/3[In])-1, respectively . It was generally observed that for CuInS2 single
crystals good p-type behavior (ρ ~1-5 Ωcm, µ ~ 15-20 cm2/Vs) could be obtained by
annealing in a sulfur overpressure, and good n-type characteristics (ρ ~1 Ωcm, µ ~ 100-200 cm2/Vs), by annealing in indium or Cu + In with a minimum S pressure [27, 28]. Similar behavior was observed for CuInS2 films. Excess-sulfur films were generally p-type
while sulfur-deficient and indium-rich films were n-type .
Table 2.3. Summary of the defect levels of donors and acceptors reported for CuInS2.
Defect nature Defect assignment Ionization energy
(eV) Refs Acceptor VCu 0.10 [34-37] Acceptor VIn 0.15 [10, 28, 38-40] Donor VS (or InCu) 0.035 [35, 38-41] Donor Ini (or InCu) 0.072 [38, 39] Donor InCu 0.145 (0.16) [33, 35]
The observed behavior of the conducting type of CuInS2 can be understood based on
the predicted defect energies and on the ternary Cu-In-S phase diagram. In table 2.3, the defect levels of donors and acceptors reported for CuInS2 are summarized. A schematic
Cu-In-S ternary phase diagram indicating the expected defects and majority-carrier type in the region around stoichiometric CuInS2, derived from the Cu-In-Se system , is shown
in Fig. 2.3. S-rich films containing both Cu and In vacancies (acceptors) should yield strongly p-type films. In-rich layers with a sulfur deficiency should be dominated by both antisite (In-on-Cu-site) donor defects and S vacancies (also donors), yielding the observed, highly conductive n-type layers. In Cu-rich films with sulfur contents near the pseudobinary tie line, antisite (Cu-on-In-site) acceptor defects and acceptors contributed by In vacancies are predominant, leading to a strong p-type conducting as observed. On the
other hand, In-rich layers with sulfur contents near the pseudobinary tie line, governed by antisite (In-on-Cu site) donor defects and Cu vacancies (acceptors), two oppositely charged defects, may be expected to behave, heavily compensated, intrinsic or high-resistivity n- or
p-type conducting. In table 2.4, the electrical transport data of CuInS2 single crystals and
thin films reported so far are collected in terms of resistivity, carrier concentration, and Hall mobility.
Fig. 2.3. A schematic Cu-In-S ternary phase diagram indicating the expected defects and majority-carrier type in the region around stoichiometric CuInS2, derived from the Cu-In-Se system .
Table 2.4. Summary of electrical transport data, such as resistivity, carrier concentration, and Hall mobility, reported for CuInS2 single crystals and thin films.
Single crystals Films
ρ (Ωcm) n,p (cm-3) µ (cm2/Vs) ρ (Ωcm) n,p (cm-3) µ (cm2/Vs) n-type 1 3.7×1012-3.5×1017 100-200 0.01-4.9×104 4.0×1012-1019 0.032-240 p-type 1-5 5.2×1015-1.0×1017 15-20 0.01-500 1013-1020 0.025-95
and film deposition
As outlined in the introduction, so far, various methods have been performed to produce CuInS2 (CIS) films, including a rapid thermal process , single source evaporation ,
coevaporation from elemental sources , sulfurization of metallic precursors , chemical vapor deposition , sputtering , electrodeposition , and spray pyrolysis , etc. Compared to other techniques, sputtering has, in principle, the advantage of simple and flexible control of the film stoichiometry over a large scale at relatively low cost. In practice, the sputtering technique has already been utilized to produce a wide range of functional materials in industry. In this study, we therefore choose reactive sputtering technique for the deposition of CIS thin films. In the present chapter, we first introduce briefly the basic working principle of RF reactive sputtering and the specific setup used in this work, then describe the typical sputter parameters for the deposition of CIS films.
3.1 Sputtering principle and apparatus
Sputter deposition is one of the physical vapor deposition (PVD) techniques. In the basic sputtering process, the source material, named target, is bombarded by energetic positive ions (inert gas such as argon ions) generated in a glow discharge plasma situated in the front of the target. The bombardment process causes the removal, i.e., “sputtering”, of target atoms, which may then condense in a thin film on a desired substrate. The positively charged gas ions from the plasma are attracted and accelerated towards the target by the electric field obtained as a result of applying a negative potential on the target with respect to the substrate electrode. Thus the source electrode for the target is known as cathode, and the substrate electrode anode.
If the applied potential between the cathode (target) and anode (substrate) is constant with time, the process is called DC (direct-current) sputtering, by which highly electrical conductive materials like metallic films can be well-deposited. It is, however, hardly possible to deposit insulating films by DC sputtering, since the poor conductivity of the target material leads to accumulation of positive charges on the target (cathode), which in turn eliminates the intentionally applied negative potential on the target. For deposition of insulating films, RF sputtering is designed, which avoids the positive charging on the
target by applying an alternating potential instead. If, during the sputter process, in addition to the inert sputtering gas (working gas), a reactive component (e.g. O2 or N2) is
introduced, we generally define the process – RF reactive sputtering, which is just the case for the present study.
Fig. 3.1. Schematic representations of (a) the RF reactive sputter system, and (b) the two targets used in this study, a Cu-In inlay target (Cu: red; In: gray) with an area ratio Cu/In of approximately 1, and a Cu-In alloy target with Cu/In of 9/11.
Fig. 3.1 illustrates schematically the RF reactive sputter apparatus used in this work for depositing CIS films. The complete sputter system basically consists of five parts: a RF generator, a matching unit, the deposition chamber, a pumping system, and the gas inlet system. Each part plays a specific role in the sputter process as outlined below.
•RF generator: The RF generator is used to create a dense glow discharge between the target (cathode) and the substrate (anode), and to cause a bias potential to build up on the target surface. The positively charged ions in the plasma are, by several orders of magnitude, heavier than the negatively charged electrons. While the electrons can follow and neutralize positive charges, the ions no longer follow the high frequency switching, particularly in the radio freqency (13.56 MHz) regime, leading to an unaltered negative self biasing of the target relative to the substrate, as shown in Fig. 3.2. The negative bias potential of the traget with respect to the substrate results in the ion bombardment, i.e., sputtering of the target. A SG-1250 RF generator with a maximum output of 1250 W was used in our sputter apparatus.
•Deposition chamber: The deposition chamber (sputter chamber) is a glass-walled vacuum station, equipped mainly with water cooled target holder (cathode electrode) at the top and back shields, adjustable water cooled substrate holder (anode electrode),
and accessory base rings. In our sputter apparatus, the distance between the target and substrate is approximately 8 cm.
•Matching unit: A matching unit is designed and mounted normally on top of the sputter chamber, to achieve an efficient energy transfer from the RF generator at a nominal load of approximately 50 Ω, to the sputter chamber, which has a considerably higher impedance.
•Pumping system: There are two pumps, a mechanical rough pump and a molecular turbopump, together with a liquid nitrogen trap, connected to our sputter system. A pressure of 10-5 Pa could be achieved.
•Gas inlet system: There are several mass flow controllers (MFC) installed in our sputter apparatus, which enables individual control of the flow rates of the individual gases.
Fig. 3.2. The target, substrate, and plasma potentials in a RF sputter process as a function of time, and the self bias potentials of the target, UT, and substrate, US, with respect to the plasma. There is an unaltered
negative potential between the target and the substrate.
3.2 Film deposition
During the course of this study, CIS films were prepared on bare, Mo-, or ZnO-coated float glass and single crystalline sapphire substrates by RF reactive sputtering with the setup described above. Two kinds of targets, a Cu-In inlay target and a Cu-In alloy target, were used for sputter deposition of CIS films. Both targets were originally 4 inches in diameter and 0.25 inches thick, as illustrated in Fig. 3.1 (b). The Cu-In inlay target with an area ratio Cu/In of approximately unity resulted in films of good crystallinity and morphology, however, highly off-stoichiometry (extremely Cu-rich). Using instead a Cu-In alloy target
with Cu/In of 9/11, nearly stoichiometric CuInS2 films were produced. In this thesis, if no
special notation is given, the films are sputtered with the Cu-In alloy target.
Prior to film deposition the sputter chamber was normally evacuated to about 10-4 Pa. Immediately before the sputter process, the bare or coated float glass or sapphire substrates were cleaned ultrasonically in organic solvents: acetone and methanol, each for about 5 min, then dried by compressed nitrogen gas. Even for sapphire substrates used for epitaxial growth of CIS films, no chemical etching or heating treatments were further performed before film growth.
Fig. 3.3. (a) The plasma generated by a mixture gas Ar/H2S, (b) the plasma generated by pure H2S gas.
Pre-sputtering, i.e., cleaning of the target was generally performed with an argon (purity: 99.999%) plasma for 10 min. H2S (purity: 98.0%) was introduced as reactive gas.
At the beginning of this work, we sputtered CIS films in an Ar/H2S mixture atmosphere.
Cu-In secondary phases were usually found incorporated in the films sputtered in such an atmosphere. By introducing H2S solely as both reactive and working gas during sputtering,
nearly stoichiometric films with pure CIS phase were deposited. Interestingly, while the color of the Ar/H2S plasma is pink-like, the plasma generated by pure H2S is more like ice
blue (see Fig. 3.3). As will be discussed in the following chapters, the deposition parameters have a strong influence on the properties of the sputtered films. In table 3.1, the general sputter parameters used in the present study are summarized.
Table 3.1. Summary of typical sputter parameters for deposition of CIS films in this work. Substrate Power (W) Substrate temperature (°C) H2S flow rate (sccm) p(H2S) (Pa) Ar flow rate (sccm) p(total) (Pa) Deposition rate (nm/min) Float glass 200 400 10-17.5 1.04-1.87×10-1 1.5-2.3 2.0 - 2.67×10-1 -Float glass 200 400 17.5-29 1.87-2.93×10-1 - 1.87-3.20×10-1 ~ 32 Float glass 200 500 25-35 2.67-3.73×10-1 - 2.67-3.73×10-1 -Float glass 300 400 20-40 1.93 - 4.0×10-1 - 1.93 - 4.0×10-1 -Float glass 300 500 40-45 4.0 - 4.53×10-1 - 4.0 - 4.53×10-1 -Sapphire 200 500 30 3.07×10-1 - 3.07×10-1 ~ 40
For comparative studies, several binary compound and elemental films, such as Cu2S,
CuS, Cu-In, metallic Cu films, were prepared as well using the same sputter setup. Typical sputter parameters for these films are outlined in table 3.2, along with the typical deposition rates. Metallic Mo layers, typical back contacts for CIS-based solar cells, were sputtered also in this work, with the parameters given in table 3.2.
Table 3.2. Typical sputter conditions for Cu-In, Cu2S, CuS, Cu, and Mo films in this study.
Film Target Power (W) Substrate temperature (°C) H2S flow rate (sccm) p(H2S) (Pa) Ar flow rate (sccm) p(total) (Pa) Deposition rate (nm/min) Cu-In Cu-In alloy a)100-200 RT - - 4.2 1.6×10-1 ~16 (200W)
Cu2S Cu b) 100-300 RT-500 3.5-10 0.4-1.07×10-1 2.3 1.25-1.93×10-1 21~27
CuS Cu 50-100 RT-200 10 1.07×10-1 2.3 1.93×10-1 ~ 20
Cu Cu 300 RT - - 4.2 1.6×10-1 ~ 24
Mo Mo c) 200-300 RT - - 4.2 1.6×10-1 ~11 (200W)
Several methods have been used to characterize the sputtered films in this study. For structural characterization, the techniques such as X-ray diffraction (XRD), X-ray reflectometry (XRR), and transmission electron microscopy (TEM) were employed. The surface and morphology analyses were accomplished by photoemission spectroscopy (XPS and UPS) and secondary ion mass spectrometry (SIMS), atomic force microscopy (AFM) and scanning electron microscopy (SEM), including energy-dispersive X-ray analysis (EDX), respectively. SIMS and EDX were additionally utilized to examine the composition of the films in the bulk. The optical and electrical properties of the films were determined by optical transmission and Hall effect measurements, respectively. In this chapter, the main principles of these techniques, and the specific instruments and typical measuring conditions (parameters) used in this work are briefly described.
4.1 Structural characterization methods (XRD,
XRR, and TEM)
4.1.1 X-ray diffraction
X-ray diffraction is a powerful non-destructive method for material characterization, by which the crystal structure, orientation, and grain size can be determined. The characterization is usually carried out with a typical X-ray wavelength that is comparable to the interatomic distance in a crystal (~ 0.1 nm). When X-rays impinge on a crystal, the individual atoms act as secondary radiation emitters and cause interference analogous to the diffraction of light from a grating. Constructive interferences give the diffraction peaks according to Bragg’s law,
λ θ n
2 , (4.1) which relates the distance between a set of planes, d, in a crystal and the angle, θ, at which these planes will diffract X-rays of a particular wavelength, λ.
In an X-ray diffractometer the X-ray source is usually in fixed position and the sample stage and the detector can be rotated individually or simultaneously. According to the
rotation possibility of the sample stage and detector, the X-ray diffractometers are generally classified as powder diffractometers, which are suited for probing powder or polycrystalline samples, and four-circle diffractometers, particularly designed for single crystalline specimens or texture analysis of oriented polycrystalline samples.
X-ray powder diffraction
Fig. 4.1 shows the schematic representation of a standard Bragg-Brentano powder diffractometer, Siemens D5000, in the First Physics Institute of Giessen University. In such a powder diffractometer, the sample stage and detector can only rotate in the same plane, along the same axis (diffractometer axis) perpendicular to the figure and located at the center of the sample stage, and thus it is also called two-circle diffractometer. Depending on the coupling of the sample and/or detector rotations during diffraction measurements, three scan modes, i.e., θ-2θ scan, rocking curve, and detector scan are used for structural characterizations.
Fig. 4.1 Schematic representation of Bragg-Brentano powder diffractometer, Siemens D5000.
In the case of θ-2θ scan, when the sample is rotated the detector follows the sample motion in the same direction around the diffractometer axis by twice the speed of the sample. This technique is also called locked-coupled scan. In θ-2θ scan, the reflections from the planes parallel to the substrate surface are detected. This allows to determine the orientation along the growth direction of an epitaxial layer or preferentially oriented polycrystalline film with respect to the substrate. In addition, the full width at half maximum (FWHM) of the peak, ∆(2θ) (in radians), is a measure of the size, b, of the
grains in a polycrystalline film or the mosaic blocks in an epitaxial layer, as described by Scherrer’s formula : ) cos( ) 2 ( 89 . 0 θ θ λ ⋅ ∆ = b , (4.2)
where θ is the Bragg angle and λ the X-ray wavelength. When the grains are larger than the film thickness, h, then b=h.
In the rocking curve mode, known also as ω scan for four-circle diffractometer, the sample is “rocked” by a small angle around the Bragg angle θ with the detector remaining in a fixed position (2θ). The half width of the rocking curve is a direct measure of the range of orientation present in the crystal, thus, it is commonly used for evaluating the out-of-plane ordering of the epitaxial layers.
In detector scan (2θ scan), while the sample is fixed the detector rotates alone. For grazing incidence X-ray diffraction (GIXRD), the detector scan mode is always adopted. While the X-ray beam irradiates the sample at a constant grazing angle, e.g., 1.0°, the detector counts the diffracted signals in a set 2θ range.
Fig. 4.2 Schematic illustration of the configuration of a four-circle X-ray diffractometer.
For assessment of the quality of an epitaxial layer or texture analysis of a preferentially oriented polycrystalline film, a four-circle X-ray diffractometer is necessarily required. In a four-circle X-ray diffractometer, the sample can rotate in three planes, i.e., ω, φ, and χ-circles, as indicated in Fig. 4.2, plus the 2θ-circle for detector rotation, the diffractometer is thus called four-circle diffractometer.
A material is called textured if the grains are aligned in a preferred orientation along certain directions. The textured state of a material (typically in thin films) can be viewed as an intermediate state in between a completely randomly distributed polycrystalline powder and a perfectly oriented single crystal. For texture analysis, a polefigure, typically Chi-Phi mapping, is carried out measuring the intensity of a given reflection (2θ is constant) at a large number of different angular orientations of the sample, i.e., various settings of Chi and Phi. Normally one measures all Phi (in-plane rotation) values for a given angle of Chi (azimuth angle), then changes Chi and repeats the process until the whole range of Chi and Phi is covered. For different specific purpose, one can perform also the Phi-2θ mapping while keeping Chi at a fixed angle, as we will demonstrate in chapter 6.
Under grazing incidence conditions, with an incident angle of typically 1° or lower, the incident X-ray beam is nearly parallel to the film surface, thus the reflections generated from the planes perpendicular to the surface are detected. By grazing incidence ω or φ-scans, the in-plane orientation of the films with respect to the substrates can be directly determined.
For characterization of the sputtered polycrystalline films on float glass substrates, we used a Bragg-Brentano powder diffractometer, Siemens D5000, which is schematically illustrated in Fig. 4.1, with Cu Kα (λ= 0.15418 nm) radiation and a scintillation detector.
The X-ray tube was typically operated at a voltage of 40 kV and a current of 20 mA. A Siemens-Stoe AED2 four circle-diffractometer with Mo Kα (λ =0.71069 Å)
radiation, in the Institute of Inorganic and Analytical Chemistry of Giessen University, was employed for characterization of epitaxially grown thin films on sapphire. X-ray diffraction measurements of thick CIS films sputtered with a thin buffer, grown quasi-epitaxially on sapphire, were mainly carried out at the Institute of Experimental Physics of Magdeburg University. For normal θ-2θ scans a standard Bragg-Brentano diffractometer, Siemens D5000, with a Cu Kα radiation and graphite secondary monochromator was used.
A Seifert/FPM URD6/TZ6 four-circle X-ray diffractometer, with a Cu Kα X-ray source,
Barthels primary monochromator, Eulerian cradle sample stage, and a Ge(220) secondary analyzer was applied for the Phi-Chi scan (polefigure) measurements. Grazing incidence diffraction was accomplished with a Seifert/FPM URD6 four-circle diffractometer,
equipped with a Cu Kα radiation source, a primary vertical Soller collimator (0.15°), a
vertical translation sample holder, and a secondary vertical Soller collimator and LiF analyzer.
Further information on X-ray diffraction techniques is referred to [1-3].
4.1.2 X-ray reflectometry
X-ray reflectometry is now a well suited method for the study of surfaces and thin layers, since it provides a wealth of information on thickness and interfacial properties on the nanometer scale, like layer thickness, the layer’s electronic densities, surface and interface roughness and roughness morphology.
The measurement principle is based on the fact that the refractive index for all elements and compounds at short wavelengths of X-rays (~ 0.1 nm) is slightly smaller than 1:
β δ i
n= 1− − (4.3) with δ describing the dispersion and β the absorption of a material at a certain wavelength. Consequently, external total reflection occurs when X-rays hit a sample at a grazing incidence angle. As the refractive index for the interesting wavelengths is very close to 1 (δ and β are positive and have values typically of the order 10-6), total reflection occurs at
very small incidence angles of the order of several tenths of a degree. The exact value for the critical angle of total reflection ΘC can, in principle, be used to determine the density of
a deposited film or the density at the surface of a bulk material according to: δ 2 = ΘC (4.4) with 2 ) ( 2π λ ρ δ Z f A r Na e ′ + = , (4.5)
where Na is the Avogadro's number, re the classical electron radius, ρ the mass density, A
the atomic mass, Z the atomic number, f ′ the dispersion correction, and λ the X-ray wavelength.
At incidence angles slightly above the critical angle of total reflection of a thin film, some intensity penetrates into the film and is partly reflected at the interface between the film and the substrate. The radiation reflected from the interface interferes with that reflected directly from the film surface. Upon changing the incidence angle, the two
contributions give rise to interference fringes whose spacing is characteristic for the film thickness. The equation
2 2 2 2 2 4d m C m λ + Θ = Θ (4.6)
gives the position of the mth interference maximum as a function of the total reflection angle of ΘC, with wavelength λ and the film thickness d, and therefore offers the
possibility to determine the film thickness from the position of interference maxima .
In this study the XRR measurements were performed with the same diffractometer used for X-ray powder diffraction, equipped with a modified sample stage, designed specially for XRR by Bruker AXS. In addition to the main parts for XRD, a controllable beam stop and a metal absorber for reducing the too high intensity of the totally reflected X-rays at lower than the critical angle are added, as illustrated in Fig. 4.3. The XRR measurements, in grazing incidence θ-2θ scan mode, of our sputtered CIS films were typically carried out from 2θ = 0.35° to 3.0° with a scan step of 0.002°. Afterwards, the program “Refsim” was used to simulate the experimental curve, to obtain thickness, surface density, and roughness of the layers and roughness of the interfaces between the layers and substrates. Although the described setup allows the measurement of film thickness up to about 300 nm for very smooth surface, we can, in practice, measure only films with thickness less than 100 nm, due to the rough surfaces of the sputtered CIS films.
Fig. 4.3. Illustration of the setup for X-ray reflectometry.
More detailed theoretical background on X-ray reflectivity and introduction to practical X-ray reflectometry techniques can be found in [4, 6-12].
4.1.3 Transmission electron microscopy
Transmission electron microscopy is a versatile tool capable of characterizing the internal structure of a wide range of materials . TEM characterization enables not only the direct imaging of the microstructure, but also the identification of the phases present in the specimen by either electron diffraction or spectroscopic chemical analysis. The results obtained from a typical TEM characterization offers a better understanding of the relation between the microstructure and properties of the materials.
There are various operation modes of the electron microscope. The bright field (BF) mode is usually used to image grains and defect structures within the specimen. It can also reveal secondary phases such as precipitates or inclusions. Similar in purpose to the BF technique, the dark field (DF) imaging mode uses the specific Bragg diffracted electrons to image the region from which they originated. The DF mode enables the connection between the crystallographic information and specific regions or phases in the sample. The principal function of the electron diffraction technique is to determine the crystallographic structure of the material being analyzed. By placing an aperture in the image plane, then projecting the diffraction pattern of that image onto the recording plate, the selected area diffraction pattern (SADP) is obtained.
For more detailed description of TEM techniques and practical applications in material research refer to [13-16].
4.2 Surface and morphology characterization
methods (XPS, UPS, SIMS, SEM, and AFM)
4.2.1 Photoemission spectroscopy (XPS and UPS)
X-ray photoelectron spectroscopy (XPS), known as electron spectroscopy for chemical analysis (ESCA), and ultraviolet photoelectron spectroscopy (UPS), are extreme surface-sensitive methods for chemical and electronic characterization of materials. Surface analysis by XPS or UPS is accomplished by irradiating a sample in vacuum with monoenergetic soft X-rays or ultraviolet radiation and analyzing the energy of the detected electrons. Mg Kα (1253.6 eV) or Al Kα (1486.6 eV) X-rays and He I (21.21 eV) or He II
(40.84 eV) radiations are usually used for XPS and UPS, respectively. These photons interact with atoms in the surface region of the sample, causing electrons to be emitted by
the photoelectric effect. The emitted electrons have measured kinetic energies, EK given by: s B K hν E E = − −φ , (4.7) where hv is the photon energy, EB is the binding energy of the atomic orbital from which
the electron originates, and φs is the spectrometer work function. The spectrum is obtained
as a plot of the number of detected electrons per energy interval versus their kinetic energy. Since each element has a unique set of binding energies, XPS can be used to identify the elements in the surface qualitatively referring to the peak positions, and determine quantitatively the concentration of each element, Cx, according to its peak height
or peak area, with the formula:
∑= = i i i x x i i x x S I S I n n C / / , (4.8)
where I is the number of emitted photoelectrons, and S the atomic sensitivity factor. The chemical shifts, i.e., variations in the elemental binding energies, caused by differences in the chemical potential and polarizability of compounds, can be used to identify the chemical state of the materials. The UPS spectrum is sensitive to the valence band region, thus, gives insight in the density of filled states at and near the surface and allows the extraction of the valence band structure of the material.
photoemission spectroscopy experiments in the present study were carried out using a VG ESCALAB system with photon energy of 1253.6 eV (Mg Kα) for XPS and 21.21 eV
(He I) for UPS, respectively, at a base pressure of about 2×10-10 mbar. Detailed XPS and
UPS investigation on the sputtered CIS films in this work is discussed elsewhere . More information about photoemission background and practical application of ESCA can be found for example in ref. [18-21].
4.2.2 Secondary ion mass spectrometry
Secondary ion mass spectrometry is frequently used to characterize the surface and near surface (~ 30 µm) region of solids and the surface of some liquids. The technique uses a beam of energetic (0.5-20 keV) primary ions, commonly Ar+, O2+, Cs+, and Ga+, to sputter
the sample surface, producing ionized secondary particles that are detected using a mass spectrometer (magnetic sector-, quadrupole-, or time-of-flight-spectrometers). Three types of SIMS data are generally achievable: mass spectra, depth profiles, and ion images.
A mass spectrum, describing the secondary ion intensities of the species detected as a function of mass, is produced by sputtering a sample while the mass spectrometer scans the
mass range. From the arising masses in the spectrum one recognizes the elements represented, thus, general information about the composition as well as impurities included in the sample surface is achieved. Depth profiles are obtained if, instead of scanning the mass spectrometer as the sputtering continues, one or more masses are monitored sequentially by switching rapidly among masses. Via a depth profile, one receives information about the concentration of selected elements into the depth, and thus the depth homogeneity of the sample is examined. When a mode of data collection analogous to SEM is operated for SIMS, element-specific images or maps can be generated by recording the secondary ions emitted from the sample that are detected with a mass spectrometer. Ion images of SIMS generally provide information about the uniformity of the lateral element distribution at the surface or in the bulk of the sample.
In the present work, SIMS measurements were accomplished with the plant MIQ 56A (CAMECA/Riber), using argon or oxygen primary ions. Mass spectra were recorded to survey the impurities at the surface of the films. Depth profiles were carried out to examine the depth homogeneity of the films.
For deeper insight into secondary ion mass spectrometry techniques see [22-24].
4.2.3 Scanning electron microscopy
Due to its versatility and the wide range of information it can provide, the scanning electron microscope is often the preferred starting tool for analytical microscopy. In SEM a finely focused electron beam scans the sample along closely spaced lines. As a result of the interaction between the electron beam and the specimen, a variety of signals, mainly secondary plus backscattered electrons and X-rays, are produced . Using special detectors, these signals can be collected giving specific information about the irradiated volume.
Secondary electrons are emitted from the atoms occupying the top surface (~ 5 nm) and produce a readily interpretable image, the contrast of which is determined by the sample surface morphology. Backscattered electrons are primary beam electrons that are 'reflected' from atoms in the solid. As its contrast is determined by the atomic number of the elements in the sample, the image generated by backscattered electrons represents the distribution of different chemical phases in the sample.
Interaction of the primary electron beam with atoms in the sample causes shell transitions which result in the emission of X-rays. Detection and measure of the characteristic X-rays enables elemental analysis, i.e., so-called energy dispersive X-ray analysis (EDX). EDX provides rapid qualitative, or with adequate standards, quantitative analysis of elemental composition within a sampling depth of 1-2 microns. X-rays may
also be used to form maps or line profiles, showing the elemental distribution in a sample surface.
In the present study, a Philips XL20 SEM was applied to observe the surface as well as cross-sectional morphology of the films. The images were produced by detecting the secondary electrons, with a typical acceleration voltage of 10 or 30 kV. An EDX system, using a SiLi-detector with an ultrathin window (UTW), integrated with the SEM setup was used to analyze the composition of the sputtered films. Typical electron acceleration voltage for EDX operation is 10 kV.
General information on working principles of SEM and its versatile applications in materials science can be found for instance in [25-27].
4.2.4 Atomic force microscopy
The atomic force microscope probes the surface of a sample with a microfabricated tip (~10 nm in diameter) mounted on a flexible cantilever (100-200 µm long). Forces between the tip and the sample surface (van der Waals forces or Pauli exclusion forces, etc.) cause the cantilever to bend, or deflect. A detector measures the cantilever deflection as the tip is scanned over the sample. The measured cantilever deflections allow a computer to generate a map of surface topography with resolutions down to atomic and nanoscales. The lateral and vertical movements of the tip or sample are controlled by piezoelectric transducers and a feedback loop that produces voltage differences proportional to the movement.
The atomic force microscope can be operated under two different conditions, in air or in a vacuum, and via two primary modes, contact or non-contact, to produce surface imaging and three-dimensional profiling. Surface imaging by AFM, with a lateral resolution down to about 3 nm, can be used to determine the roughness, grain size, and features on the nanoscale and resolve individual holes, defects (such as pinholes), and atomic clusters on the sample surface. Three-dimensional profiling probes samples in real, three-dimensional space with vertical resolutions up to 0.01 nm. Via storage of digital information, the three-dimensional image may be manipulated and enhanced with color, filtered, enlarged, and displayed from any altitude or azimuth. AFM is suitable to investigate a wide range of materials, including insulators, semiconductors and electrical conductors.
In the course of this study, we used a home-built AFM, in addition to SEM, to characterize the surface morphology of the sputtered films. The AFM was operated in air in the contact mode. Two- as well as three-dimensional images were recorded to provide a
general view on the film surfaces and determine quantitatively the surface roughness and grain size of the films.
A review of AFM techniques can be found in .
4.3 Optical transmission
The optical properties of the sputtered CIS films were characterized by optical transmission spectrum measurements. The transmission spectra were recorded with a Varian 2300 spectrophotometer typically in the wavelength range of 350-2500 nm at room temperature.
According to the transmission spectra, the absorption coefficient α of the films was evaluated with the expression
T = −α , (4.9) which neglects the surface and multiple reflection effects. Here T is the transmission coefficient and t the film thickness. In this study, the thickness of the films was measured either directly by XRR or, for thick films, estimated via multiplying the sputter time by the average deposition rate determined by XRR.
Following the usual theoretical analysis , the energy dependent absorption coefficient α(hν) can be expressed by the relation for the allowed direct transition as
2 / 1 ) ( ) (hv =A hν −E α , (4.10) where A is a constant, hν the photon energy, and E refers to the direct band edge. By extrapolating along the linear portion of the α2 versus hν curve to the hν axis, the direct
bandgaps of the films, represented by the intercept at the hν axis, were deduced.
4.4 Hall effect measurements
The electrical properties of our sputtered CIS films were characterized by Hall effect measurements. Hall effect experiments were conducted with a Van der Pauw technique. Plated silver or pre-sputtered molybdenum were used for contacts. Typically the carrier concentration, resistivity, and Hall mobility, in dependence on temperature ranging from 77 to 400 K were measured to evaluate the electrical properties of the films. Hall effect investigation on the electrical properties of the sputtered CIS films in this study has been described in detail elsewhere . Detailed measuring procedures for the CIS films and
more basic knowledge about Hall effect technique can be found there and references therein.
RF reactive sputtering
Deposition of CuInS2 film by sputtering usually consists of two steps. At first a precursor
of Cu/In stacked multilayers, a Cu-In alloy film or Cu-In-S film is sputtered using, respectively, Cu and In elemental targets [1-3], a Cu-In inlay target , or mixed powder target of Cu2S and In2S3 . In a second step, the sputtered precursor is annealed or
sulfurized in a H2S or elemental S atmosphere. For industrial application, the
simplification of the process is one of the key issues for low cost. The aim of this work is thus set to develop a one-stage process for the deposition of CuInS2 films by RF reactive
sputtering . Along with this prospect, we first tried to sputter CuInS2 films using a Cu-In
inlay target and H2S gas. Films with good crystallinity and morphology, however, highly
off-stoichiometry (extremely Cu-rich) have been obtained . By utilizing a Cu-In alloy target, nearly stoichiometric CuInS2 films can be sputtered but additionally in-situ
annealing is necessary due to the deficient H2S flow amount during sputtering . With an
extended H2S mass flow controller, we finally succeeded in deposition of CIS films by RF
reactive sputtering in one step .
To optimize the sputtering process, we first investigated systematically the influence of sputter parameters on the film properties. Then, we focused our studies on the surface characterization of the sputtered films. Its properties are significant for achieving high-efficiency CIS film solar cells. Although stoichiometric CIS films can be sputtered in one step, we have found that post-growth treatments have significant influences on properties of the sputtered films, e.g., enhancement of the structural and optical properties by post-growth annealing, modification of the film surfaces by chemical etching. Detailed studies on these issues are the three main parts of the following chapter .
5.1 Influence of the sputter parameters on the
properties of CuInS2
5.1.1 Influence of the H2
S flow during sputtering
As usual, we began with argon as working gas for providing the plasma, introducing simultaneously the reactive gas H2S for sputtering. In Fig. 5.1 XRD spectra of four films
sputtered at 400 °C with different H2S flows are presented. Films (a), (b) and (c) were
sputtered in a H2S/Ar atmosphere, while film (d) was sputtered solely in H2S. Besides
peaks of CIS there are some additional peaks originating from Cu-In alloy phases, such as Cu11In9, Cu4In, and CuIn, coexisting in the films sputtered with argon. We normalized the
maximum intensity of each spectrum and chose the same scale, thus, the relative abundance of phases present in the films is represented by the intensity ratio of peaks from different phases. As can be seen, with a fixed Ar flow amount of 2.3 sccm but increasing the H2S flow rate from 10 to 15 sccm, the secondary Cu-In phases are gradually depressed.
In order to keep the total gas pressure during sputtering as low as possible, and since, we thought H2S could be used as working gas as effectively as argon due to the comparable
atomic mass, we decided to use H2S solely as both working and reactive gas during
sputtering . With a H2S flow rate of 20 sccm, 2.13×10-1 Pa in partial pressure, pure
CuInS2 phase films with a chalcopyrite structure were obtained (see Fig. 5.1(d)). Hereafter,
all the studied films are sputtered with solely H2S gas if no specific notation is given.
20 30 40 50 60 70 80 CuIn Cu4In Cu11In9 (a) 2 Θ (degree) (b) (116/312) (204/220) (c) (d) (112) (224) X R D In te ns ity ( a. u.)
Fig. 5.1. XRD spectra of CIS films sputtered at 400°C and 200 W with different flow rates of H2S and Ar,
(a) f(H2S) = 10 sccm, f(Ar) = 2.3 sccm; (b) f(H2S) = 12.5 sccm, f(Ar) = 2.3 sccm; (c) f(H2S) = 15 sccm, f(Ar)
= 2.3 sccm; (d) f(H2S) = 20 sccm, f(Ar) = 0 sccm.
These films have a highly (112) preferential orientation, since only the (112) and (224) diffraction peaks which originate from the same series of lattice planes of CIS were detected. It is useful to estimate quantitatively the preferred structural (112) orientation. According to the method for evaluating the magnitude of the preferred orientation factor f
employed in CuInSe2 thin films and other materials [10, 11], we define the preferred
orientation factor f(112) for the (112) plane as ) 1 /( ) (p p0 p0 f = − − (5.1) with
∑= Inn n Ihkl p 2 / and =
∑* 2 0 Inn n / Ihkl p , (5.2) where Ihkl is the measured intensity of (hkl) peak of the films, I the standard intensity for*hkl
the randomly distributed powder CuInS2, and n the diffraction order. For an increasing
degree of orientation, p increases from the value p0 for a nonoriented material to 1 for a
totally oriented sample so that the orientation factor f increases from 0 (nonoriented) to 1 (totally oriented). Applying this formula, a preferential orientation factor f(112) as high as approximately 0.96 has been deduced for films sputtered only with H2S .
20 30 40 50 60 70 80 90 (a) CuIn Cu11In9 f(H2S)=20 sccm XR D Int ensit y (a. u.) 2 Θ (degree) (b) (228/424) (420) (316/332) f(H2S)=25 sccm (c) (224) (116/312) (204/220) (004/200) (112) f(H2S)=28 sccm (d) f(H 2S)=30 sccm (e) (400) f(H2S)=33 sccm (f) S f(H2S)=35 sccm
Fig. 5.2. XRD spectra of CIS films sputtered at 500°C and 200 W with different flow rates of H2S.
A H2S flow of 20 sccm is sufficient to sputter pure CuInS2 phase film at 400 °C but not
enough to avoid Cu-In alloy phases coexisting in the films sputtered at a substrate temperature of 500 °C . Fig. 5.2 shows the XRD spectra of films sputtered at 500 °C with a power of 200 W but different H2S flows. When the H2S flow during sputtering
increased to 25 sccm, the secondary Cu-In phases were suppressed, and nearly pure CuInS2
more H2S is needed to avoid Cu-In alloy minor phases. However, when the H2S flow is
above 30 sccm, there are some additional peaks arising from elemental S present (see Fig. 5.2 (f)). Therefore, the suitable H2S flow amount for sputtering at 500 °C and 200 W is in
the range between 25 and 30 sccm, in contrast to a H2S flow rate of 20-29 sccm which is
suited for sputtering at 400 °C and 200 W, as listed in Table 5.1.
22 23 24 25 26 27 28 29 30 47.0 47.5 H2S flow amount (sccm) 2 4 6 8 10 12 0.12 1000/T (K-1 ) 48.0 48.5 49.0 49.5 50.0 50.5 51.0 (a) S concentrat ion (at%) 0.16 0.20 0.24 0.28 f(H2S)=23 sccm f(H2S)=26 sccm f(H2S)=29 sccm R esistivit y ( Ω cm) 450 300 150 (b) T (K)
Fig. 5.3. (a) S concentration in the films sputtered at 400° and 200 W with different H2S flows and (b) the
temperature dependence of the resistivity of these films.
With a fixed sputter power and substrate temperature, a higher H2S flow during
sputtering, as expected, results in a higher S content in the sputtered films. Fig. 5.3 (a) shows the S content in the films (determined by EDX) sputtered at a RF power of 200 W and a substrate temperature of 400 °C with different H2S flows. The S atomic
concentration increases from 47.9% to 50.2% as the H2S flow is increased from 23 sccm to
29 sccm. In Fig. 5.3 (b), the corresponding resistivities of these films are compared. The aged films (exposed to air for several weeks) are p-type as determined by Hall effect measurements. The higher S content reduces the S vacancies (favorable for n-type) in the films, thus enhancing the p-type conducting of the films and, consequently, leads to slightly higher hole concentrations and lower resistivities of the films .
5.1.2 Influence of the substrate temperature
We heated the substrates to different temperatures while keeping the other parameters constant to investigate the influence of the substrate temperature on the film properties. In Fig. 5.4 XRD spectra of two films sputtered with a same power of 200 W but different substrate temperatures of 400 and 500°C, respectively, are presented for comparison. A logarithmic scale is used for the XRD intensity in order to see more details. A higher